#------------------------------------------------------------------------------
#$Date: 2016-02-16 22:30:59 +0200 (Tue, 16 Feb 2016) $
#$Revision: 176467 $
#$URL: svn://www.crystallography.net/cod/cif/4/33/39/4333991.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4333991
loop_
_publ_author_name
'T. Thao Tran'
'P. Shiv Halasyamani'
_publ_contact_author_address
;
Department of Chemistry
University of Houston
Houston, Texas
77204-5003
USA
;
_publ_contact_author_email       psh@uh.edu
_publ_contact_author_fax         1-713-743-0796
_publ_contact_author_name        'P. Shiv Halasyamani'
_publ_contact_author_phone       1-832-775-8696
_publ_section_title
;
 New Fluoride Carbonates: Centrosymmetric KPb2(CO3)2F and
 Noncentrosymmetric K2.70Pb5.15(CO3)5F3
;
_journal_name_full               'Inorganic Chemistry'
_journal_page_first              2466
_journal_page_last               2473
_journal_paper_doi               10.1021/ic302357h
_journal_volume                  52
_journal_year                    2013
_chemical_absolute_configuration unk
_chemical_formula_sum            'C5 F3 K2.7 O15 Pb5.15'
_chemical_formula_weight         1529.65
_chemical_name_systematic
;
 ?
;
_space_group_IT_number           187
_symmetry_cell_setting           hexagonal
_symmetry_space_group_name_Hall  'P -6 2'
_symmetry_space_group_name_H-M   'P -6 m 2'
_atom_sites_solution_hydrogens   none
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                120.00
_cell_formula_units_Z            1
_cell_length_a                   5.3123(5)
_cell_length_b                   5.3123(5)
_cell_length_c                   18.6203(17)
_cell_measurement_reflns_used    2002
_cell_measurement_temperature    301(2)
_cell_measurement_theta_max      27.35
_cell_measurement_theta_min      2.19
_cell_volume                     455.07(7)
_computing_cell_refinement       'SAINT v7.12A (Bruker-Nonius, 2004)'
_computing_data_collection       'APEX2 v1.0-27 (Bruker-Nonius, 2005)'
_computing_data_reduction        'SAINT v7.12A (Bruker-Nonius, 2004)'
_computing_structure_refinement  'SHELXL v6.12 (G.M. Sheldrick, 2001)'
_computing_structure_solution    'SHELXS v6.12 (G.M. Sheldrick, 2001)'
_diffrn_ambient_temperature      301(2)
_diffrn_detector_area_resol_mean 4K
_diffrn_measured_fraction_theta_full 0.993
_diffrn_measured_fraction_theta_max 0.993
_diffrn_measurement_device_type  'Bruker APEX II CCD'
_diffrn_measurement_method       CCD
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0478
_diffrn_reflns_av_sigmaI/netI    0.0127
_diffrn_reflns_limit_h_max       0
_diffrn_reflns_limit_h_min       -5
_diffrn_reflns_limit_k_max       6
_diffrn_reflns_limit_k_min       0
_diffrn_reflns_limit_l_max       23
_diffrn_reflns_limit_l_min       0
_diffrn_reflns_number            2776
_diffrn_reflns_theta_full        27.35
_diffrn_reflns_theta_max         27.35
_diffrn_reflns_theta_min         2.19
_diffrn_standards_decay_%        0.0
_exptl_absorpt_coefficient_mu    48.194
_exptl_absorpt_correction_T_max  0.9863
_exptl_absorpt_correction_T_min  0.5665
_exptl_absorpt_correction_type   empirical
_exptl_absorpt_process_details   'SAINT v7.12A'
_exptl_crystal_colour            Colorless
_exptl_crystal_density_diffrn    5.582
_exptl_crystal_description       column
_exptl_crystal_F_000             651
_exptl_crystal_size_max          0.10
_exptl_crystal_size_mid          0.10
_exptl_crystal_size_min          0.05
_refine_diff_density_max         1.404
_refine_diff_density_min         -2.320
_refine_diff_density_rms         0.208
_refine_ls_abs_structure_details 'Flack H D (1983), Acta Cryst. A39, 876-881'
_refine_ls_abs_structure_Flack   0.012(18)
_refine_ls_extinction_coef       0.0068(5)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   1.159
_refine_ls_hydrogen_treatment    none
_refine_ls_matrix_type           full
_refine_ls_number_parameters     44
_refine_ls_number_reflns         470
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.159
_refine_ls_R_factor_all          0.0210
_refine_ls_R_factor_gt           0.0207
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0423P)²+0.3300P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0598
_refine_ls_wR_factor_ref         0.0600
_reflns_number_gt                467
_reflns_number_total             470
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            ic302357h_si_003_2.cif
_cod_data_source_block           K2.70Pb5.15(CO3)5F3
_cod_original_formula_sum        'C5 F3 K2.70 O15 Pb5.15'
_cod_database_code               4333991
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-y, x-y, z'
'-x+y, -x, z'
'x, y, -z'
'-y, x-y, -z'
'-x+y, -x, -z'
'-y, -x, z'
'-x+y, y, z'
'x, x-y, z'
'-y, -x, -z'
'-x+y, y, -z'
'x, x-y, -z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
Pb1 Pb 0.6667 0.3333 0.5000 0.0154(3) Uani 1 12 d S
Pb2 Pb 0.6667 0.3333 0.24818(5) 0.0154(2) Uani 1 6 d S
Pb3 Pb 0.3333 0.6667 0.12609(4) 0.0173(3) Uani 1 6 d S
K1 K 0.3333 0.6667 0.37958(18) 0.0206(11) Uani 1 6 d S
K2 K 0.6667 0.3333 0.0000 0.0198(9) Uani 0.70 12 d SP
Pb4 Pb 0.6667 0.3333 0.0000 0.0198(9) Uani 0.15 12 d SP
F1 F 0.643(3) 0.357(3) 0.3687(5) 0.025(5) Uiso 0.33 2 d SP
F2 F 0.3333 0.6667 0.0000 0.020(3) Uani 1 12 d S
C1 C 1.0000 0.0000 0.5000 0.022(9) Uani 1 12 d S
O1 O 1.1408(10) 0.282(2) 0.5000 0.025(2) Uani 1 4 d S
C2 C 1.0000 0.0000 0.2666(11) 0.011(4) Uani 1 6 d S
O2 O 1.1405(7) 0.2811(15) 0.2678(3) 0.0227(16) Uani 1 2 d S
C3 C 0.0000 1.0000 0.1077(12) 0.015(5) Uani 1 6 d S
O3 O -0.1393(7) 0.7214(15) 0.1066(3) 0.0222(16) Uani 1 2 d S
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
F F 0.0171 0.0103 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
K K 0.2009 0.2494 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Pb Pb -3.3944 10.1111 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
F1 Pb1 F1 170.0(15) 6_666 3_665
F1 Pb1 F1 175.0(7) 6_666 2_655
F1 Pb1 F1 175.0(7) 3_665 5_656
F1 Pb1 F1 170.0(15) 2_655 5_656
F1 Pb1 F1 175.0(7) 6_666 .
F1 Pb1 F1 175.0(7) 5_656 .
F1 Pb1 F1 175.0(7) 3_665 4_556
F1 Pb1 F1 175.0(7) 2_655 4_556
F1 Pb1 F1 170.0(15) . 4_556
F1 Pb1 O1 89.55(7) 6_666 2_645
F1 Pb1 O1 89.55(7) 3_665 2_645
F1 Pb1 O1 85.9(6) 2_655 2_645
F1 Pb1 O1 85.9(6) 5_656 2_645
F1 Pb1 O1 94.6(7) . 2_645
F1 Pb1 O1 94.6(7) 4_556 2_645
F1 Pb1 O1 85.9(6) 6_666 3_775
F1 Pb1 O1 85.9(6) 3_665 3_775
F1 Pb1 O1 94.6(7) 2_655 3_775
F1 Pb1 O1 94.6(7) 5_656 3_775
F1 Pb1 O1 89.55(7) . 3_775
F1 Pb1 O1 89.55(7) 4_556 3_775
O1 Pb1 O1 120.000(1) 2_645 3_775
F1 Pb1 O1 85.9(6) 6_666 .
F1 Pb1 O1 85.9(6) 3_665 .
F1 Pb1 O1 89.55(7) 2_655 .
F1 Pb1 O1 89.55(7) 5_656 .
F1 Pb1 O1 94.6(7) . .
F1 Pb1 O1 94.6(7) 4_556 .
O1 Pb1 O1 49.8(4) 2_645 .
O1 Pb1 O1 70.2(4) 3_775 .
F1 Pb1 O1 94.6(7) 6_666 3_665
F1 Pb1 O1 94.6(7) 3_665 3_665
F1 Pb1 O1 85.9(6) 2_655 3_665
F1 Pb1 O1 85.9(6) 5_656 3_665
F1 Pb1 O1 89.55(7) . 3_665
F1 Pb1 O1 89.55(7) 4_556 3_665
O1 Pb1 O1 70.2(4) 2_645 3_665
O1 Pb1 O1 169.8(4) 3_775 3_665
O1 Pb1 O1 120.000(1) . 3_665
F1 Pb1 O1 89.55(7) 6_666 2_655
F1 Pb1 O1 89.55(6) 3_665 2_655
F1 Pb1 O1 94.6(7) 2_655 2_655
F1 Pb1 O1 94.6(7) 5_656 2_655
F1 Pb1 O1 85.9(6) . 2_655
F1 Pb1 O1 85.9(6) 4_556 2_655
O1 Pb1 O1 169.8(4) 2_645 2_655
O1 Pb1 O1 49.8(4) 3_775 2_655
O1 Pb1 O1 120.000(1) . 2_655
O1 Pb1 O1 120.000(1) 3_665 2_655
F1 Pb1 O1 94.6(7) 6_666 1_455
F1 Pb1 O1 94.6(7) 3_665 1_455
F1 Pb1 O1 89.55(6) 2_655 1_455
F1 Pb1 O1 89.55(6) 5_656 1_455
F1 Pb1 O1 85.9(6) . 1_455
F1 Pb1 O1 85.9(6) 4_556 1_455
O1 Pb1 O1 120.000(2) 2_645 1_455
O1 Pb1 O1 120.000(1) 3_775 1_455
O1 Pb1 O1 169.8(4) . 1_455
O1 Pb1 O1 49.8(4) 3_665 1_455
O1 Pb1 O1 70.2(4) 2_655 1_455
F1 Pb2 O2 81.76(15) 3_665 2_645
F1 Pb2 O2 77.8(7) 2_655 2_645
F1 Pb2 O2 87.2(8) . 2_645
F1 Pb2 O2 77.8(7) 3_665 .
F1 Pb2 O2 81.76(15) 2_655 .
F1 Pb2 O2 87.2(8) . .
O2 Pb2 O2 49.2(3) 2_645 .
F1 Pb2 O2 77.8(7) 3_665 3_775
F1 Pb2 O2 87.2(8) 2_655 3_775
F1 Pb2 O2 81.76(15) . 3_775
O2 Pb2 O2 118.20(6) 2_645 3_775
O2 Pb2 O2 69.6(3) . 3_775
F1 Pb2 O2 87.2(8) 3_665 3_665
F1 Pb2 O2 77.8(7) 2_655 3_665
F1 Pb2 O2 81.76(15) . 3_665
O2 Pb2 O2 69.6(3) 2_645 3_665
O2 Pb2 O2 118.20(6) . 3_665
O2 Pb2 O2 161.3(3) 3_775 3_665
F1 Pb2 O2 81.76(15) 3_665 2_655
F1 Pb2 O2 87.2(8) 2_655 2_655
F1 Pb2 O2 77.8(7) . 2_655
O2 Pb2 O2 161.3(3) 2_645 2_655
O2 Pb2 O2 118.20(6) . 2_655
O2 Pb2 O2 49.2(3) 3_775 2_655
O2 Pb2 O2 118.20(6) 3_665 2_655
F1 Pb2 O2 87.2(8) 3_665 1_455
F1 Pb2 O2 81.76(15) 2_655 1_455
F1 Pb2 O2 77.8(7) . 1_455
O2 Pb2 O2 118.20(6) 2_645 1_455
O2 Pb2 O2 161.3(3) . 1_455
O2 Pb2 O2 118.20(6) 3_775 1_455
O2 Pb2 O2 49.2(3) 3_665 1_455
O2 Pb2 O2 69.6(3) 2_655 1_455
F2 Pb3 O3 82.25(14) . 2_675
F2 Pb3 O3 82.25(14) . 3_565
O3 Pb3 O3 70.1(3) 2_675 3_565
F2 Pb3 O3 82.25(14) . .
O3 Pb3 O3 48.7(3) 2_675 .
O3 Pb3 O3 118.21(6) 3_565 .
F2 Pb3 O3 82.25(14) . 3_455
O3 Pb3 O3 118.21(6) 2_675 3_455
O3 Pb3 O3 161.1(3) 3_565 3_455
O3 Pb3 O3 70.1(3) . 3_455
F2 Pb3 O3 82.25(14) . 1_655
O3 Pb3 O3 118.21(6) 2_675 1_655
O3 Pb3 O3 48.7(3) 3_565 1_655
O3 Pb3 O3 161.1(3) . 1_655
O3 Pb3 O3 118.21(6) 3_455 1_655
F2 Pb3 O3 82.25(14) . 2_665
O3 Pb3 O3 161.1(3) 2_675 2_665
O3 Pb3 O3 118.21(6) 3_565 2_665
O3 Pb3 O3 118.21(6) . 2_665
O3 Pb3 O3 48.7(3) 3_455 2_665
O3 Pb3 O3 70.1(3) 1_655 2_665
O2 K1 O2 68.3(2) 2_655 1_455
O2 K1 O2 68.3(2) 2_655 3_675
O2 K1 O2 68.3(2) 1_455 3_675
O2 K1 O1 101.3(2) 2_655 2_655
O2 K1 O1 142.97(9) 1_455 2_655
O2 K1 O1 142.97(9) 3_675 2_655
O2 K1 O1 142.97(9) 2_655 1_455
O2 K1 O1 101.3(2) 1_455 1_455
O2 K1 O1 142.97(9) 3_675 1_455
O1 K1 O1 64.9(3) 2_655 1_455
O2 K1 O1 142.97(9) 2_655 3_675
O2 K1 O1 142.97(9) 1_455 3_675
O2 K1 O1 101.3(2) 3_675 3_675
O1 K1 O1 64.9(3) 2_655 3_675
O1 K1 O1 64.9(3) 1_455 3_675
O2 K1 F1 67.83(15) 2_655 2_665
O2 K1 F1 126.4(3) 1_455 2_665
O2 K1 F1 67.83(15) 3_675 2_665
O1 K1 F1 75.31(17) 2_655 2_665
O1 K1 F1 132.4(2) 1_455 2_665
O1 K1 F1 75.31(17) 3_675 2_665
O2 K1 F1 67.83(15) 2_655 .
O2 K1 F1 67.83(15) 1_455 .
O2 K1 F1 126.4(3) 3_675 .
O1 K1 F1 75.31(17) 2_655 .
O1 K1 F1 75.31(17) 1_455 .
O1 K1 F1 132.4(2) 3_675 .
F1 K1 F1 119.50(5) 2_665 .
O2 K1 F1 126.4(3) 2_655 3_565
O2 K1 F1 67.83(15) 1_455 3_565
O2 K1 F1 67.83(15) 3_675 3_565
O1 K1 F1 132.4(2) 2_655 3_565
O1 K1 F1 75.31(17) 1_455 3_565
O1 K1 F1 75.31(17) 3_675 3_565
F1 K1 F1 119.50(5) 2_665 3_565
F1 K1 F1 119.50(5) . 3_565
O2 K1 F1 66.2(3) 2_655 3_675
O2 K1 F1 126.7(2) 1_455 3_675
O2 K1 F1 70.2(3) 3_675 3_675
O1 K1 F1 73.1(3) 2_655 3_675
O1 K1 F1 131.9(2) 1_455 3_675
O1 K1 F1 76.8(3) 3_675 3_675
F1 K1 F1 3.4(5) 2_665 3_675
F1 K1 F1 116.2(5) . 3_675
F1 K1 F1 122.9(5) 3_565 3_675
O2 K1 F1 70.2(4) 2_655 2_655
O2 K1 F1 66.2(3) 1_455 2_655
O2 K1 F1 126.7(2) 3_675 2_655
O1 K1 F1 76.8(3) 2_655 2_655
O1 K1 F1 73.1(3) 1_455 2_655
O1 K1 F1 131.9(2) 3_675 2_655
F1 K1 F1 122.9(5) 2_665 2_655
F1 K1 F1 116.2(5) 3_565 2_655
F1 K1 F1 119.60(4) 3_675 2_655
O2 K1 F1 66.2(3) 2_655 3_665
O2 K1 F1 70.2(4) 1_455 3_665
O2 K1 F1 126.7(2) 3_675 3_665
O1 K1 F1 73.1(3) 2_655 3_665
O1 K1 F1 76.8(3) 1_455 3_665
O1 K1 F1 131.9(2) 3_675 3_665
F1 K1 F1 116.2(5) 2_665 3_665
F1 K1 F1 122.9(5) 3_565 3_665
F1 K1 F1 112.9(10) 3_675 3_665
O3 K2 O3 96.1(3) 1_655 4_655
O3 K2 O3 140.93(11) 1_655 5_665
O3 K2 O3 70.8(2) 4_655 5_665
O3 K2 O3 70.8(2) 1_655 2_665
O3 K2 O3 140.93(11) 4_655 2_665
O3 K2 O3 96.1(3) 5_665 2_665
O3 K2 O3 140.93(11) 1_655 6
O3 K2 O3 70.8(2) 4_655 6
O3 K2 O3 70.8(2) 5_665 6
O3 K2 O3 140.93(11) 2_665 6
O3 K2 O3 70.8(2) 1_655 3
O3 K2 O3 140.93(11) 4_655 3
O3 K2 O3 140.93(11) 5_665 3
O3 K2 O3 70.8(2) 2_665 3
O3 K2 O3 96.1(3) 6 3
O3 K2 F2 70.47(5) 1_655 1_655
O3 K2 F2 70.47(5) 4_655 1_655
O3 K2 F2 131.97(14) 5_665 1_655
O3 K2 F2 131.97(14) 2_665 1_655
O3 K2 F2 70.47(5) 6 1_655
O3 K2 F2 70.47(5) 3 1_655
O3 K2 F2 70.47(5) 1_655 .
O3 K2 F2 70.47(5) 4_655 .
O3 K2 F2 70.47(5) 5_665 .
O3 K2 F2 70.47(5) 2_665 .
O3 K2 F2 131.97(14) 6 .
O3 K2 F2 131.97(14) 3 .
F2 K2 F2 120.0 1_655 .
O3 K2 F2 131.97(14) 1_655 1_545
O3 K2 F2 131.97(14) 4_655 1_545
O3 K2 F2 70.47(5) 5_665 1_545
O3 K2 F2 70.47(5) 2_665 1_545
O3 K2 F2 70.47(5) 6 1_545
O3 K2 F2 70.47(5) 3 1_545
F2 K2 F2 120.0 1_655 1_545
F2 K2 F2 120.0 . 1_545
Pb2 F1 Pb1 169.5(16) . .
Pb2 F1 K1 99.5(9) . .
Pb1 F1 K1 91.0(7) . .
Pb2 F1 K1 90.6(5) . 1_655
Pb1 F1 K1 83.6(4) . 1_655
K1 F1 K1 122.9(5) . 1_655
Pb2 F1 K1 90.6(5) . 1_545
Pb1 F1 K1 83.6(4) . 1_545
K1 F1 K1 122.9(5) . 1_545
K1 F1 K1 112.9(10) 1_655 1_545
Pb3 F2 Pb3 180.0 4 .
Pb3 F2 K2 90.0 4 1_455
Pb3 F2 K2 90.0 . 1_455
Pb3 F2 K2 90.0 4 1_565
Pb3 F2 K2 90.0 . 1_565
K2 F2 K2 120.0 1_455 1_565
Pb3 F2 K2 90.0 4 .
Pb3 F2 K2 90.0 . .
K2 F2 K2 120.0 1_455 .
K2 F2 K2 120.0 1_565 .
O1 C1 O1 120.000(2) . 3_765
O1 C1 O1 120.000(2) . 2_645
O1 C1 O1 120.000(4) 3_765 2_645
C1 O1 Pb1 95.1(2) . 1_655
C1 O1 Pb1 95.1(2) . .
Pb1 O1 Pb1 169.8(4) 1_655 .
C1 O1 K1 128.31(16) . 4_656
Pb1 O1 K1 86.83(14) 1_655 4_656
Pb1 O1 K1 86.83(14) . 4_656
C1 O1 K1 128.31(16) . 1_655
Pb1 O1 K1 86.83(14) 1_655 1_655
Pb1 O1 K1 86.83(14) . 1_655
K1 O1 K1 103.4(3) 4_656 1_655
O2 C2 O2 119.97(6) 3_765 2_645
O2 C2 O2 119.97(6) 3_765 .
O2 C2 O2 119.97(6) 2_645 .
C2 O2 Pb2 95.0(2) . 1_655
C2 O2 Pb2 95.0(2) . .
Pb2 O2 Pb2 161.3(3) 1_655 .
C2 O2 K1 131.4(10) . 1_655
Pb2 O2 K1 92.59(14) 1_655 1_655
Pb2 O2 K1 92.59(14) . 1_655
O3 C3 O3 119.97(7) 3_465 .
O3 C3 O3 119.97(7) 3_465 2_675
O3 C3 O3 119.97(7) . 2_675
C3 O3 K2 132.9(11) . 1_455
C3 O3 Pb3 95.2(2) . .
K2 O3 Pb3 92.16(15) 1_455 .
C3 O3 Pb3 95.2(2) . 1_455
K2 O3 Pb3 92.17(15) 1_455 1_455
Pb3 O3 Pb3 161.1(3) . 1_455
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Pb1 F1 2.454(9) 6_666
Pb1 F1 2.454(9) 3_665
Pb1 F1 2.454(9) 2_655
Pb1 F1 2.454(9) 5_656
Pb1 F1 2.454(9) .
Pb1 F1 2.454(9) 4_556
Pb1 O1 2.6668(9) 2_645
Pb1 O1 2.6668(9) 3_775
Pb1 O1 2.6668(9) .
Pb1 O1 2.6668(9) 3_665
Pb1 O1 2.6668(8) 2_655
Pb1 O1 2.6668(8) 1_455
Pb2 F1 2.254(10) 3_665
Pb2 F1 2.254(10) 2_655
Pb2 F1 2.254(10) .
Pb2 O2 2.6918(11) 2_645
Pb2 O2 2.6918(11) .
Pb2 O2 2.6918(11) 3_775
Pb2 O2 2.6918(11) 3_665
Pb2 O2 2.6918(11) 2_655
Pb2 O2 2.6918(11) 1_455
Pb3 F2 2.3478(8) .
Pb3 O3 2.6926(11) 2_675
Pb3 O3 2.6926(11) 3_565
Pb3 O3 2.6926(11) .
Pb3 O3 2.6926(11) 3_455
Pb3 O3 2.6926(11) 1_655
Pb3 O3 2.6926(11) 2_665
K1 O2 2.735(7) 2_655
K1 O2 2.735(7) 1_455
K1 O2 2.735(7) 3_675
K1 O1 2.858(7) 2_655
K1 O1 2.858(7) 1_455
K1 O1 2.858(6) 3_675
K1 F1 2.86(3) 2_665
K1 F1 2.86(3) .
K1 F1 2.86(3) 3_565
K2 O3 2.669(7) 1_655
K2 O3 2.669(7) 4_655
K2 O3 2.669(7) 5_665
K2 O3 2.669(7) 2_665
K2 O3 2.669(7) 6
K2 O3 2.669(7) 3
K2 F2 3.0671(3) 1_655
K2 F2 3.0671(3) .
K2 F2 3.0671(3) 1_545
F2 Pb3 2.3478(8) 4
F2 K2 3.0671(3) 1_455
F2 K2 3.0671(3) 1_565
C1 O1 1.296(10) .
C1 O1 1.296(9) 3_765
C1 O1 1.296(10) 2_645
O1 Pb1 2.6668(9) 1_655
O1 K1 2.858(6) 4_656
O1 K1 2.858(6) 1_655
C2 O2 1.293(7) 3_765
C2 O2 1.293(7) 2_645
C2 O2 1.293(7) .
O2 Pb2 2.6917(11) 1_655
O2 K1 2.735(7) 1_655
C3 O3 1.282(7) 3_465
C3 O3 1.282(7) .
C3 O3 1.282(7) 2_675
O3 K2 2.669(7) 1_455
O3 Pb3 2.6926(11) 1_455
